LMucko/crystallography-open-database huggingface dataset:
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517928
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47305(14)
_cell_length_b                   7.47305(14)
_cell_length_c                   7.47305(14)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    160
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.344(14)
_diffrn_ambient_temperature      160
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2531(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.60
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.20
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.78
_refine_ls_R_I_factor            1.08
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_160K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.34(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517928
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517929
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47296(13)
_cell_length_b                   7.47296(13)
_cell_length_c                   7.47296(13)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    140
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.328(13)
_diffrn_ambient_temperature      140
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2532(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.60
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.19
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.77
_refine_ls_R_I_factor            1.09
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_140K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.33(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517929
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517930
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47497(16)
_cell_length_b                   7.47497(16)
_cell_length_c                   7.47497(16)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    260
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.665(15)
_diffrn_ambient_temperature      260
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2499(3)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 3 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.69
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.18
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.76
_refine_ls_R_I_factor            1.08
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_260K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.67(3)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517930
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517931
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47257(14)
_cell_length_b                   7.47257(14)
_cell_length_c                   7.47257(14)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    60
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.263(14)
_diffrn_ambient_temperature      60
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2539(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.61
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.20
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.79
_refine_ls_R_I_factor            1.09
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_60K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.26(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517931
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517932
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47552(15)
_cell_length_b                   7.47552(15)
_cell_length_c                   7.47552(15)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    280
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.757(15)
_diffrn_ambient_temperature      280
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2489(3)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.68
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.22
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.80
_refine_ls_R_I_factor            1.08
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_280K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.76(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517932
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517933
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47270(9)
_cell_length_b                   7.47270(9)
_cell_length_c                   7.47270(9)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    40
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.285(9)
_diffrn_ambient_temperature      40
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.072
_exptl_crystal_density_diffrn    4.25366(16)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.56
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.20
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.79
_refine_ls_R_I_factor            1.12
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_40K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.285(15)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517933
Intrinsic Isotropic Near-Zero Thermal Expansion in Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
Liu, Youquan; Mei, Dajiang; Wang, Naizheng; Molokeev, Maxim S.; Jiang, Xingxing; Lin, Zheshuai; ACS applied materials & interfaces 12 (2020) 38435–38440; doi:10.1021/acsami.0c12351

data_4517934
_publ_section_title
;
 Intrinsic Isotropic Near-Zero Thermal Expansion in
 Zn<sub>4</sub>B<sub>6</sub>O<sub>12</sub>X (X = O, S, Se).
;
_journal_issue                   34
_journal_name_full               'ACS applied materials &amp; interfaces'
_journal_page_first              38435
_journal_page_last               38440
_journal_paper_doi               10.1021/acsami.0c12351
_journal_volume                  12
_journal_year                    2020
_chemical_formula_moiety
;
B6 O13 Zn4
;
_chemical_formula_sum            'B6 O13 Zn4'
_chemical_formula_weight         534.42
_chemical_name_mineral
;
;
_space_group_IT_number           217
_space_group_name_Hall           'I -4 2 3'
_space_group_name_H-M_alt        'I -4 3 m'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'I -4 2 3'
_symmetry_space_group_name_H-M   'I -4 3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.47339(13)
_cell_length_b                   7.47339(13)
_cell_length_c                   7.47339(13)
_cell_measurement_reflns_used    104
_cell_measurement_temperature    180
_cell_measurement_theta_max      45
_cell_measurement_theta_min      5
_cell_volume                     417.400(13)
_diffrn_ambient_temperature      180
_diffrn_measurement_device_type
;
D8 ADVANCE Bruker
;
_diffrn_radiation_monochromator  none
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type
;
 Cu K\a~1~~2~
;
_exptl_absorpt_coefficient_mu    14.073
_exptl_crystal_density_diffrn    4.2525(2)
_exptl_crystal_description       cylinder
_pd_char_colour
;
colourless
;
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        90
_pd_meas_2theta_range_min        10
_pd_meas_scan_method             step
_pd_proc_ls_pref_orient_corr
;
Anisotropic model of PO. Spherical harmonics 2 ordrer.
 Jarvinen (1993). Application of symmetrized harmonics expansion to correction
of the preferred orientation effect. - J. Appl. Cryst. 26 p525-531.
;
_pd_proc_ls_profile_function     PearsonVII
_pd_proc_ls_prof_R_factor        4.58
_pd_proc_ls_prof_wR_expected     1.24
_pd_proc_ls_prof_wR_factor       7.15
_pd_proc_number_of_points        4000
_pd_spec_mount_mode              reflection
_refine_ls_goodness_of_fit_all   5.74
_refine_ls_R_I_factor            1.07
_refine_ls_shift/su_max          0.01000
_cod_data_source_file            ZBO_180K.cif
_cod_data_source_block           a
_cod_depositor_comments
'Adding full bibliography for 4517906--4517952.cif.'
_cod_original_cell_volume        417.40(2)
_cod_original_sg_symbol_Hall
;
I -4 2 3
;
_cod_original_sg_symbol_H-M      I-43m
_cod_original_formula_sum
;
B6 O13 Zn4
;
_cod_database_code               4517934